title: Novel bioactive materials with different mechanical properties.
abstract: Some ceramics, such as Bioglass, sintered hydroxyapatite, and glass-ceramic A-W, spontaneously bond to living bone. They are called bioactive materials and are already clinically used as important bone substitutes. However, compared with human cortical bone, they have lower fracture toughness and higher elastic moduli. Therefore, it is desirable to develop bioactive materials with improved mechanical properties. All the bioactive materials mentioned above form a bone-like apatite layer on their surfaces in the living body, and bond to bone through this apatite layer. The formation of bone-like apatite on artificial material is induced by functional groups, such as Si-OH, Ti-OH, Zr-OH, Nb-OH, Ta-OH, -COOH, and PO(4)H(2). These groups have specific structures revealing negatively charge, and induce apatite formation via formations of an amorphous calcium compound, e.g., calcium silicate, calcium titanate, and amorphous calcium phosphate. These fundamental findings provide methods for preparing new bioactive materials with different mechanical properties. Tough bioactive materials can be prepared by the chemical treatment of metals and ceramics that have high fracture toughness, e.g., by the NaOH and heat treatments of titanium metal, titanium alloys, and tantalum metal, and by H(3)PO(4) treatment of tetragonal zirconia. Soft bioactive materials can be synthesized by the sol-gel process, in which the bioactive silica or titania is polymerized with a flexible polymer, such as polydimethylsiloxane or polytetramethyloxide, at the molecular level to form an inorganic-organic nano-hybrid. The biomimetic process has been used to deposit nano-sized bone-like apatite on fine polymer fibers, which were textured into a three-dimensional knit framework. This strategy is expected to ultimately lead to bioactive composites that have a bone-like structure and, hence, bone-like mechanical properties.
authors.affiliation: Department of Material Chemistry, Faculty of Engineering, Graduate School of Engineering, Kyoto University, Yoshida, Sakyo-ku, 606-8501, Kyoto, Japan
authors.forename: Tadashi
authors.initials: T
authors.lastname: Kokubo
authors.forename: Hyun-Min
authors.initials: HM
authors.lastname: Kim
authors.forename: Masakazu
authors.initials: M
authors.lastname: Kawashita
mesh_terms: D000818:Animals; D001672:Biocompatible Materials / Q000138:chemical synthesis / Q000737:chemistry*; D032701:Biomimetics / Q000295:instrumentation / Q000379:methods / Q000639:trends; D001709:Biotechnology / Q000295:instrumentation / Q000379:methods* / Q000639:trends; D001861:Bone Regeneration / Q000502:physiology; D016723:Bone Remodeling / Q000502:physiology*; D018786:Bone Substitutes / Q000138:chemical synthesis / Q000737:chemistry*; D002130:Calcium Phosphates; D002516:Ceramics / Q000138:chemical synthesis / Q000737:chemistry*; D017886:Durapatite / Q000737:chemistry; D006801:Humans; D008420:Manufactured Materials; D016348:Osseointegration / Q000502:physiology; D012038:Regeneration / Q000502:physiology; D023822:Tissue Engineering / Q000295:instrumentation / Q000379:methods* / Q000639:trends
chemical_list: D001672:Biocompatible Materials; D018786:Bone Substitutes; D002130:Calcium Phosphates; C519480:amorphous calcium phosphate; D017886:Durapatite